#------------------------------------------------------------------------------
#$Date: 2023-05-05 02:25:31 +0200 (Fri 05 de May de 2023) $
#$Revision: 283091 $
#$URL: svn://www.crystallography.net/cod/cif/7/13/13/7131377.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7131377
loop_
_publ_author_name
'Yoshino, Haruka'
'Saigo, Masaki'
'Miyata, Kiyoshi'
'Onda, Ken'
'Pirillo, Jenny'
'Hijikata, Yuh'
'Kosaka, Wataru'
'Miyasaka, Hitoshi'
_publ_section_title
;
 Unprecedented highly efficient photoluminescence in a phosphorescent
 Ag(I) coordination polymer.
;
_journal_issue                   31
_journal_name_full               'Chemical communications (Cambridge, England)'
_journal_page_first              4616
_journal_page_last               4619
_journal_paper_doi               10.1039/d3cc00179b
_journal_volume                  59
_journal_year                    2023
_chemical_formula_moiety         '0.25(C48 H32 Ag8 Cd4 N32)'
_chemical_formula_sum            'C12 H8 Ag2 Cd N8'
_chemical_formula_weight         592.40
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     iterative
_audit_creation_date             2022-08-09
_audit_creation_method
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_audit_update_record
;
2023-01-10 deposited with the CCDC.	2023-03-06 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 97.9890(10)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.1237(9)
_cell_length_b                   16.274(2)
_cell_length_c                   14.6035(18)
_cell_measurement_reflns_used    6905
_cell_measurement_temperature    300
_cell_measurement_theta_max      29.08
_cell_measurement_theta_min      2.50
_cell_volume                     1676.6(4)
_computing_cell_refinement       'SAINT V8.40A (?, 2016)'
_computing_data_reduction        'SAINT V8.40A (?, 2016)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'olex2.solve (Bourhis et al., 2015)'
_diffrn_ambient_temperature      300
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.951
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0304
_diffrn_reflns_av_unetI/netI     0.0184
_diffrn_reflns_Laue_measured_fraction_full 0.995
_diffrn_reflns_Laue_measured_fraction_max 0.951
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            10078
_diffrn_reflns_point_group_measured_fraction_full 0.995
_diffrn_reflns_point_group_measured_fraction_max 0.951
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.106
_diffrn_reflns_theta_min         2.503
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    3.579
_exptl_absorpt_correction_T_max  0.7458
_exptl_absorpt_correction_T_min  0.5783
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.0864 before and 0.0393 after correction. The Ratio of minimum to maximum transmission is 0.7754. The λ/2 correction factor is Not present.'
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    2.347
_exptl_crystal_description       block
_exptl_crystal_F_000             1112
_exptl_crystal_size_max          0.294
_exptl_crystal_size_mid          0.148
_exptl_crystal_size_min          0.095
_refine_diff_density_max         0.564
_refine_diff_density_min         -1.512
_refine_diff_density_rms         0.147
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.141
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     107
_refine_ls_number_reflns         2147
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.141
_refine_ls_R_factor_all          0.0213
_refine_ls_R_factor_gt           0.0198
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0246P)²+0.8346P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0472
_refine_ls_wR_factor_ref         0.0481
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1986
_reflns_number_total             2147
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d3cc00179b2.cif
_cod_data_source_block           cdag_pmd_300k
_cod_depositor_comments
'Adding full bibliography for 7131376--7131381.cif.'
_cod_database_code               7131377
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.727
_shelx_estimated_absorpt_t_min   0.419
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
2.a Aromatic/amide H refined with riding coordinates:
 C3(H3), C4(H4), C5(H5), C6(H6)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Cd1 Cd 0.500000 0.500000 0.500000 0.02314(6) Uani 1 2 d S T P . .
Ag1 Ag 0.000000 0.48667(2) 0.750000 0.03805(7) Uani 1 2 d S T P . .
Ag2 Ag 1.000000 0.67121(2) 0.750000 0.04021(8) Uani 1 2 d S T P . .
N1 N 0.3150(3) 0.48853(12) 0.61474(15) 0.0432(5) Uani 1 1 d . . . . .
N2 N 0.6955(3) 0.59847(12) 0.58342(13) 0.0410(4) Uani 1 1 d . . . . .
N3 N 0.6911(2) 0.38814(10) 0.56758(11) 0.0311(3) Uani 1 1 d . . . . .
N4 N 0.6993(3) 0.27133(12) 0.66508(14) 0.0450(4) Uani 1 1 d . . . . .
C1 C 0.2077(3) 0.48213(13) 0.66500(15) 0.0360(4) Uani 1 1 d . . . . .
C2 C 0.7993(3) 0.62996(12) 0.63791(14) 0.0345(4) Uani 1 1 d . . . . .
C3 C 0.6212(3) 0.33980(13) 0.62768(16) 0.0393(5) Uani 1 1 d . . . . .
H3 H 0.505990 0.355386 0.645427 0.047 Uiso 1 1 calc R . . . .
C4 C 0.8650(3) 0.25017(14) 0.63893(17) 0.0457(5) Uani 1 1 d . . . . .
H4 H 0.924020 0.202213 0.662601 0.055 Uiso 1 1 calc R . . . .
C5 C 0.9507(3) 0.29626(15) 0.57888(18) 0.0459(5) Uani 1 1 d . . . . .
H5 H 1.067283 0.281138 0.562238 0.055 Uiso 1 1 calc R . . . .
C6 C 0.8580(3) 0.36632(13) 0.54360(15) 0.0370(4) Uani 1 1 d . . . . .
H6 H 0.913054 0.398937 0.502309 0.044 Uiso 1 1 calc R . . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ag Ag -0.8971 1.1015 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cd Cd -0.8075 1.2024 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N1 Cd1 N1 180.0 5_666 . ?
N1 Cd1 N2 87.92(7) . 5_666 ?
N1 Cd1 N2 87.92(7) 5_666 . ?
N1 Cd1 N2 92.08(7) . . ?
N1 Cd1 N2 92.08(7) 5_666 5_666 ?
N1 Cd1 N3 89.34(7) . . ?
N1 Cd1 N3 89.34(7) 5_666 5_666 ?
N1 Cd1 N3 90.66(7) 5_666 . ?
N1 Cd1 N3 90.66(7) . 5_666 ?
N2 Cd1 N2 180.0 . 5_666 ?
N2 Cd1 N3 87.55(6) 5_666 . ?
N2 Cd1 N3 92.45(6) 5_666 5_666 ?
N2 Cd1 N3 87.56(6) . 5_666 ?
N2 Cd1 N3 92.44(6) . . ?
N3 Cd1 N3 180.0 . 5_666 ?
C1 Ag1 Ag2 92.05(6) . 1_455 ?
C1 Ag1 Ag2 92.05(6) 2_556 1_455 ?
C1 Ag1 C1 175.89(12) 2_556 . ?
N4 Ag2 Ag1 129.02(5) 3 1_655 ?
N4 Ag2 Ag1 129.02(5) 4_656 1_655 ?
N4 Ag2 N4 101.96(9) 3 4_656 ?
C2 Ag2 Ag1 71.60(5) 2_756 1_655 ?
C2 Ag2 Ag1 71.60(5) . 1_655 ?
C2 Ag2 N4 102.27(7) 2_756 3 ?
C2 Ag2 N4 100.65(7) . 3 ?
C2 Ag2 N4 100.65(7) 2_756 4_656 ?
C2 Ag2 N4 102.27(7) . 4_656 ?
C2 Ag2 C2 143.20(11) . 2_756 ?
C1 N1 Cd1 173.1(2) . . ?
C2 N2 Cd1 163.01(18) . . ?
C3 N3 Cd1 118.58(13) . . ?
C3 N3 C6 116.49(17) . . ?
C6 N3 Cd1 124.69(13) . . ?
C3 N4 Ag2 119.93(15) . 3_445 ?
C3 N4 C4 115.78(19) . . ?
C4 N4 Ag2 122.71(14) . 3_445 ?
N1 C1 Ag1 171.96(19) . . ?
N2 C2 Ag2 171.25(19) . . ?
N3 C3 N4 126.6(2) . . ?
N4 C4 C5 122.39(19) . . ?
C4 C5 C6 117.5(2) . . ?
N3 C6 C5 121.3(2) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Cd1 N1 2.279(2) 5_666 ?
Cd1 N1 2.279(2) . ?
Cd1 N2 2.3495(18) . ?
Cd1 N2 2.3495(18) 5_666 ?
Cd1 N3 2.4016(16) 5_666 ?
Cd1 N3 2.4016(16) . ?
Ag1 Ag2 3.0033(5) 1_455 ?
Ag1 C1 2.060(2) 2_556 ?
Ag1 C1 2.060(2) . ?
Ag2 N4 2.5882(19) 4_656 ?
Ag2 N4 2.5882(19) 3 ?
Ag2 C2 2.127(2) . ?
Ag2 C2 2.127(2) 2_756 ?
N1 C1 1.136(3) . ?
N2 C2 1.131(3) . ?
N3 C3 1.326(3) . ?
N3 C6 1.333(3) . ?
N4 C3 1.328(3) . ?
N4 C4 1.335(3) . ?
C4 C5 1.361(4) . ?
C5 C6 1.381(3) . ?
